Automotive Paints and CoatingsEdited byHans-Joachim Streitbergerand Karl-Friedrich D¨ ssel o
Further ReadingH. Lipowsky, E. ArpaciCopper in the Automotive Industry2007ISBN: 978-3-527-31769-1G. Pfaff (Ed.)Encyclopedia of Applied Color2009ISBN: 978-3-527-31551-2G. Buxbaum, G. Pfaff (Eds.)Industrial Inorganic PigmentsThird, Completely Revised and Extended Edition2005ISBN: 978-3-527-30363-2E. B. Faulkner, R. J. Schwartz (Eds.)High Performance PigmentsSecond, Completely Revised and Extended Edition2008ISBN: 978-3-527-31405-8S. K. Ghosh (Ed.)Functional Coatingsby Polymer Microencapsulation2006ISBN: 978-3-527-31296-2
Automotive Paints and CoatingsEdited byHans-Joachim Streitbergerand Karl-Friedrich D¨ ssel oSecond, Completely Revised and Extended Edition
The Editors All books published by Wiley-VCH are care- fully produced. Nevertheless, authors, editors,Dr. Hans-Joachim Streitberger and publisher do not warrant the informa-Market & Management tion contained in these books, including thisSustainability in Business book, to be free of errors. Readers are ad-Patronatsstr. 13 vised to keep in mind that statements, data,48165 M¨ nster u illustrations, procedural details or other itemsGermany may inadvertently be inaccurate. Library of Congress Card No.:Dr. Karl-Friedrich D¨ssel o applied forDupont Performance CoatingsChristbusch 2542285 Wuppertal British Library Cataloguing-in-Publication DataGermany A catalogue record for this book is available from the British Library.1. Edition 19952. Completely Revised and Extended Edition Bibliographic information published by the2008 Deutsche Nationalbibliothek Die Deutsche Nationalbibliothek lists this publication in the Deutsche Nationalbibli- ograﬁe; detailed bibliographic data are avail- able in the Internet at <http://dnb.d-nb.de>. 2008 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim All rights reserved (including those of trans- lation into other languages). No part of this book may be reproduced in any form – by photoprinting, microﬁlm, or any other means – nor transmitted or translated into a machine language without written permis- sion from the publishers. Registered names, trademarks, etc. used in this book, even when not speciﬁcally marked as such, are not to be considered unprotected by law. Typesetting Laserwords Private Limited, Chennai, India Printing Strauss GmbH, M¨ rlenbach o Binding Litges & Dopf GmbH, Heppenheim Cover Design Graﬁk-Design Schulz, Fußg¨ nheim o Printed in the Federal Republic of Germany Printed on acid-free paper ISBN: 978-3-527-30971-9
V Contents Preface XVII Abbreviations XIX List of Contributors XXIII1 Introduction 1 Hans-Joachim Streitberger1.1 Historic Development 11.2 Legislation 71.3 Automotive and Automotive Paint Market 92 Materials and Concepts in Body Construction 13 Klaus Werner Thomer2.1 Introduction 132.2 Methods of Body Construction 152.2.1 Monocoque Design 152.2.2 Space Frame 182.2.3 Hybrid Type of Construction 192.2.4 Modular Way of Construction 192.3 Principles of Design 202.3.1 Conventional Design 202.3.2 Design Under Consideration of Light-Weight Construction 222.3.3 Bionics 232.4 Materials 262.4.1 Steel 2126.96.36.199 General Remarks 2188.8.131.52 Low-Carbon Deep Drawing Steels 2184.108.40.206 Higher-Strength Steels 2220.127.116.11 High-Strength Steels 318.104.22.168 High-Grade (Stainless) Steels 322.214.171.124 Manganese–Boron Steels 3126.96.36.199 Light-Construction Steel with Induced Plasticity (TWIP Steel) 332.4.2 Aluminum 34Automotive Paints and Coatings. Edited by H.-J. Streitberger and K.-F. D¨ ssel oCopyright 2008 WILEY-VCH Verlag GmbH & Co. KGaA, WeinheimISBN: 978-3-527-30971-9
VI Contents 188.8.131.52 General Remark 34 184.108.40.206 Further Treatment 35 220.127.116.11 Aluminum Alloys 38 18.104.22.168 Aluminum as Light-Weight Construction Material 39 2.4.3 Magnesium 40 2.4.4 Titanium 42 2.4.5 Nonmetallic Parts – Fiber Composites 43 2.5 Manufacturing Methods 47 2.5.1 Tailored Products 47 22.214.171.124 General Remarks 47 126.96.36.199 Tailored Blanks 47 188.8.131.52 Tailored Tubes 48 184.108.40.206 Tailored Strips 48 220.127.116.11 Patchwork Blanks 48 18.104.22.168 Future 49 2.5.2 Hydroforming 49 2.5.3 Press Hardening 50 2.5.4 Metal Foam 50 2.5.5 Sandwich Structures 51 2.5.6 Roll Forming to Shape 52 2.6 Joining Methods 52 2.6.1 Bonding 53 2.6.2 Laser Welding 54 2.6.3 Others 55 22.214.171.124 Clinching 55 126.96.36.199 Riveting 56 188.8.131.52 Roller Hemming 56 2.7 Outlook 57 2.8 Surface Protection 59 2.8.1 Precoating of Sheets 59 2.8.2 Corrosion Prevention in the Design Phase 59 3 Pretreatment of Multimetal Car Bodies 61 Horst Gehmecker 3.1 Introduction 61 3.2 Car Body Construction Materials 61 3.2.1 Sheet Materials 61 3.2.2 Surface Conditions/Contaminations 63 3.3 Pretreatment Process 65 3.3.1 Sequence of Treatment 65 3.3.2 Degreasing 65 3.3.3 Activation 69 3.3.4 Zinc Phosphating 70 3.3.5 Passivation 75 3.3.6 Pretreatment of Aluminum – Steel Structures 75
Contents VII3.3.7 Pretreatment of Magnesium 763.3.8 Pretreatment of Plastic Parts 773.4 Car Body Pretreatment Lines 773.4.1 Spray Lines 803.4.2 Continuous Horizontal Spray/Dip Line 803.4.3 RoDip3 Line 803.4.4 Vario Shuttle Line 813.4.5 Other Types of Lines 823.4.6 Construction Materials 823.4.7 Details on Process Stages 8184.108.40.206 Precleaning Stage 8220.127.116.11 Spray degrease 818.104.22.168 Dip Degrease 822.214.171.124 Rinsing 8126.96.36.199 Activation 8188.8.131.52 Phosphating 8184.108.40.206 Rinsing 8220.127.116.11 Passivation 818.104.22.168 Deionized water rinsing 822.214.171.124 Entering the Electrocoat Line 853.5 Properties and Speciﬁcations of Zinc Phosphate Conversion Layers 853.6 Environmental Legislations 863.7 Outlook 864 Electrodeposition Coatings 89 Hans-Joachim Streitberger4.1 History and Introduction 894.2 Physico-chemical Basics of the Deposition Process 904.3 Data for Quality Control 954.3.1 Voltage, Current Density, Bath Temperature, and Bath Conductivity 964.3.2 Wet Film Conductivity 964.3.3 Solid Content, Solvent Content, and pH 974.4 Resins and Formulation Principles 984.4.1 General Remarks 984.4.2 Anodic Electrodeposition Paints 994.4.3 Cathodic Electrodeposition Paints 994.5 Film Performance of Cathodic Electrocoatings 1014.5.1 Physical Film Data 1014.5.2 Corrosion Protection 1024.5.3 Chip Resistance 1044.5.4 Surface Smoothness and Appearance 1054.6 Design of Cathodic Electrocoating Lines 1064.6.1 Integration into the Coating Process of Cars and Trucks 1064.6.2 Pretreatment 107
VIII Contents 4.6.3 General Functions and Equipment of an Electrocoat Line 107 4.6.4 Tanks, Filters, Heat Exchanger, and Power Supply 108 4.6.5 Replenishment and Anode Cells 111 4.6.6 Ultraﬁltration and Rinsing Zones 114 4.6.7 Baking Oven 118 4.7 Defects During Application and their Prevention 119 4.7.1 Dirt 119 4.7.2 Craters 120 4.7.3 Surface Roughness 121 4.7.4 Film Thickness/Throwing Power 122 4.7.5 Other Defects 123 4.8 Electrocoating and Similar Processes Used in Automotive Supply Industry 124 4.9 Outlook 125 5 Primer Surfacer 129 Heinrich Wonnemann 5.1 Introduction 129 5.2 Requirement Proﬁle 132 5.2.1 Legislative Requirement 132 5.2.2 Technological Requirements 133 126.96.36.199 Film Properties 133 188.8.131.52 Product Speciﬁcations 136 184.108.40.206 Application 136 5.3 Raw Materials 138 5.3.1 Resin Components 139 5.3.2 Pigments and Extenders 141 220.127.116.11 Titanium Dioxide 143 18.104.22.168 Barium Sulfate 144 22.214.171.124 Talc 144 126.96.36.199 Silicon Dioxide 145 188.8.131.52 Feldspar 146 184.108.40.206 Carbon Blacks 146 5.3.3 Additives 146 220.127.116.11 Pigment Wetting and Dispersion Additives 148 18.104.22.168 Defoaming and Deaerating Agents 148 22.214.171.124 Surfactants and Additives for Substrate Wetting 149 126.96.36.199 Rheology Additives 149 5.3.4 Solvents 150 188.8.131.52 Aromatic Hydrocarbons: Diluents/Thinners 151 184.108.40.206 Alcohols, Cellosolves, and Esters: Solvents 151 220.127.116.11 Tetralin or Pine Oil: Very High Boiling Additive Diluents 152
Contents IX5.4 Liquid Primers 1525.4.1 Formula Principles 1518.104.22.168 Application 1522.214.171.124 Rheology 1535.4.2 Manufacturing Process 1565.4.3 Application 1585.5 Powder Primer Surfacers 1605.5.1 Formula Principles 1605.5.2 Manufacturing Process 1625.5.3 Application 1665.6 Process Sequence 1705.7 Summary and Future Outlook 1716 Top Coats 175 Karl-Friedrich D¨ ssel o6.1 Introduction 1756.2 Pigments and Color 1756.3 Single-Stage Top Coats (Monocoats) 1806.4 Base Coats 1816.4.1 Base Coat Rheology 1846.4.2 Low and Medium Solids Base Coat 1856.4.3 High Solids (HS) Base Coats 1866.4.4 Waterborne Base Coats 1866.4.5 Global Conversion to Waterborne Base Coat Technology 1876.4.6 Drying of Base Coats 1896.5 Clear Coat 1896.5.1 Market 1896.5.2 Liquid Clear Coats 1906.5.2.1 One-Component (1K) Acrylic Melamine Clear Coat 1906.5.2.2 Acrylic Melamine Silane 19126.96.36.199 Carbamate-Melamine-Based 1K Clear coat 19188.8.131.52 One-Component Polyurethane (PUR) Clear Coat 19184.108.40.206 One- (and Two-) Component Epoxy Acid Clear Coat 19220.127.116.11 Two-Component (2K) Polyurethane Clear Coat 1918.104.22.168 Waterborne Clear Coat 1946.5.3 Powder Clear Coat 1956.5.4 Top Coat Performance 1922.214.171.124 Enviromental Etch 19126.96.36.199 UV Durability of Clear Coats 19188.8.131.52 Scratch Resistant Clear Coats 2016.5.4.4 Application Properties 2046.5.5 Future Developments: UV Curing 206
X Contents 6.6 Integrated Paint Processes (IPP) for Top Coat Application 208 6.6.1 Wet-On-Wet-On-Wet Application (3 Coat 1 Bake) of Primer Surfacer–Base Coat–Clear Coat 208 6.6.2 Primerless Coating Process 209 7 Polymeric Engineering for Automotive Coating Applications 211 Heinz-Peter Rink 7.1 General Introduction 211 7.2 Polyacrylic Resins for Coating Materials in the Automotive Industry 214 7.2.1 Managing the Property Proﬁle of the Polyacrylic Resins 214 7.2.2 Manufacturing Polyacrylic Resins 218 184.108.40.206 Manufacturing Polyacrylic Resins by Means of Solution Polymerization 218 220.127.116.11 Polymerization in an Aqueous Environment 222 18.104.22.168 Mass Polymerization 224 7.3 Polyester for Coating Materials for the Automotive Industry 224 7.3.1 Managing the Property Proﬁle of Polyesters 224 7.3.2 Manufacturing Polyesters 228 7.4 Polyurethane Dispersions in Coating Materials for the Automotive Industry 231 7.4.1 Managing the Property Proﬁle of Polyurethane Resins and Polyurethane Resin Dispersions 232 7.4.2 Manufacturing Polyurethane Resin Dispersions 234 7.5 Polyurethane Polyacrylic Polymers in Coating Materials for the Automotive Industry 238 7.5.1 Introduction 238 7.5.2 Managing the Property Proﬁle of Polyurethane Polyacrylic Polymers 239 7.5.3 Manufacturing Polyurethane Polyacrylic Polymers 240 7.6 Epoxy Resins 241 7.6.1 Managing the Property Proﬁle 242 7.6.2 Manufacturing Polyepoxy Resins 243 7.7 Cross-Linking Agents and Network-Forming Resins 244 7.7.1 Introduction 244 7.7.2 Cross-Linking Agents for Liquid Coating Materials 245 22.214.171.124 Melamine and Benzoguanamine Resins 245 126.96.36.199 Tris(Alkoxycarbonylamino)-1,3,5-Triazine 248 188.8.131.52 Polyisocyanates and Blocked Polyisocyanates 249 184.108.40.206 Other Cross-Linking Agents for Liquid Coating Materials 252 7.7.3 Cross-Linking Agents for Powder Coatings in the Automotive Industry 252
Contents XI8 Paint Shop Design and Quality Concepts 259 Pavel Svejda8.1 Introduction 2598.2 Coating Process Steps 2608.2.1 Pretreatment 2618.2.2 Electrocoating (EC) 2618.2.3 Sealing and Underbody Protection 2628.2.4 Paint Application 26220.127.116.11 Function Layer and Primerless Processes 2618.104.22.168 Powder 2648.2.5 Cavity Preservation 2658.3 General Layout 2668.4 Coating Facilities 2688.4.1 Process Technology 2688.4.2 Automation in the Paint Application 2622.214.171.124 Painting Robot 2708.4.3 Application Technology 27126.96.36.199 Atomizer 27188.8.131.52 Paint Color Changer 27184.108.40.206 Paint Dosing Technology for Liquid Paints 27220.127.116.11 Paint Dosing Technology for Powder Paints 2788.4.4 Paint-Material Supply 2718.104.22.168 Paint Supply Systems for the Industrial Sector 2808.4.4.2 Paint Mix Room 2808.4.4.3 Container Group 2808.4.4.4 Circulation Line System 2822.214.171.124 Basic Principles for the Design of the Pipe Width for Circulation Lines 28126.96.36.199 Paint Supply Systems for Small Consumption Quantities and Frequent Color Change 28188.8.131.52 Small Circulation Systems 28184.108.40.206 Supply Systems for Special Colors 28220.127.116.11 Voltage Block Systems 2818.104.22.168 Voltage Block Systems with Color-Change Possibility 2822.214.171.124 Installations for the High Viscosity Material Supply 2868.4.5 Conveyor Equipment 2878.5 Paint Drying 2888.6 Quality Aspects 2908.6.1 Control Technology 2908.6.1.1 Process Monitoring and Regulation 2928.6.2 Automated Quality Assurance 29126.96.36.199 Process Optimization in Automatic Painting Installations 296
XII Contents 8.7 Economic Aspects 298 8.7.1 Overall Layout 298 8.7.2 Full Automation in Vehicle Painting 298 8.7.3 Exterior Application of Metallic Base Coats with 100% ESTA High-Speed Rotation 300 8.7.4 Robot Interior Painting with High-Speed Rotation 301 9 Coatings for Plastic Parts 305 9.1 Exterior Plastics 305 Guido Wilke 9.1.1 Introduction 305 188.8.131.52 Ecological Aspects 305 184.108.40.206 Technical and Design Aspects 306 220.127.116.11 Economical Aspects 307 9.1.2 Process Deﬁnitions 307 18.104.22.168 Ofﬂine, Inline, and Online Painting 307 22.214.171.124 Process-Related Issues, Advantages, and Disadvantages 307 9.1.3 Exterior Plastic Substrates and Parts 310 126.96.36.199 Overview 310 188.8.131.52 Basic Physical Characteristics 311 184.108.40.206 Part Processing and Inﬂuence on Coating Performance 315 9.1.4 Pretreatment 315 9.1.5 Plastic-Coating Materials 318 220.127.116.11 Basic Technical Principles of Raw-Material Selection 318 18.104.22.168 Car-Body Color 320 22.214.171.124 Contrast Color and Clear Coat on Plastic Systems 324 9.1.6 Technical Demands and Testing 324 126.96.36.199 Basic Considerations 324 188.8.131.52 Key Characteristics and Test Methods 325 9.1.7 Trends, Challenges, and Limitations 329 184.108.40.206 Substrates and Parts 329 220.127.116.11 Paint Materials 330 18.104.22.168 Processes 332 9.2 Interior Plastics 334 Stefan Jacob 9.2.1 Introduction: the ‘Interior’ Concept 334 9.2.2 Surfaces and Effects 335 9.2.3 Laser Coatings 337 22.214.171.124 Substrate Requirements 339 126.96.36.199 Requirements to Be Fulﬁlled by the Paint Systems and Coating 339 188.8.131.52 Demands Expected by the Inscription Technique 340 9.2.4 Performances of Interior Coatings 341 184.108.40.206 Mechanical and Technological Demands 341 220.127.116.11 Substrates and Mechanical Adhesion 342 18.104.22.168 Ecological and Economical Requirements 343
Contents XIII22.214.171.124 Equipment for the Application of Interior Paint Systems 3449.2.5 Raw-Material Basis of Interior Paints 3469.2.6 Summary/Outlook 34710 Adhesive Bonding – a Universal Joining Technology 351 Peter W. Merz, Bernd Burchardt and Dobrivoje Jovanovic10.1 Introduction 35110.2 Fundamentals 35110.2.1 Basic Principles of Bonding and Material Performances 35126.96.36.199 Types of Adhesives 35188.8.131.52 Adhesives are Process Materials 35510.2.1.3 Advantages of Bonding 35610.2.1.4 Application 35910.2.2 Surface Preparation 35910.2.2.1 Substrates 36184.108.40.206 Adhesion 36220.127.116.11 Durability and Aging of Bonded System 36210.3 Bonding in Car Production 36610.3.1 Body Shop Bonding 36710.3.1.1 Antiﬂutter Adhesives 36710.3.1.2 Hem-Flange Bonding 36810.3.1.3 Spot-Weld Bonding 36910.3.1.4 Crash-Resistant Adhesives/Bonding 36910.3.2 Paint Shop 37010.3.3 Trim Shop 3718.104.22.168 Special Aspects of Structural Bonding in the Trim Shop 3722.214.171.124 ‘Direct Glazing’ 37126.96.36.199 Modular Design 37188.8.131.52 Other Trim Part Bondings 37210.4 Summary 37411 In-plant Repairs 377 Karl-Friedrich D¨ ssel o11.1 Repair After Pretreatment and Electrocoat Application 37711.2 Repair After the Primer Surfacer Process 37811.3 Top-Coat Repairs 37811.4 End-of-Line Repairs 38012 Speciﬁcations and Testing 38112.1 Color and Appearance 381 Gabi Kiegle-B¨ ckler o12.1.1 Visual Evaluation of Appearance 38184.108.40.206 Specular Gloss Measurement 38220.127.116.11 Visual Evaluation of Distinctness-of-Image (DOI) 38518.104.22.168 Measurement of Distinctness-of-Image 385
XIV Contents 22.214.171.124 Visual Evaluation of ‘Orange Peel’ 386 126.96.36.199 Instrumental Measurement of Waviness (Orange Peel) 388 188.8.131.52 The Structure Spectrum and its Visual Impressions 390 184.108.40.206 Outlook of Appearance Measurement Techniques 392 12.1.2 Visual Evaluation of Color 393 220.127.116.11 Solid Colors 393 18.104.22.168 Metallic and Interference Colors 397 22.214.171.124 Color Measurement of Solid Colors 398 126.96.36.199 Color Measurement of Metallic and Interference Coatings 401 188.8.131.52 Typical Applications of Color Control in the Automotive Industry 402 184.108.40.206 Color Measurement Outlook 403 12.2 Weathering Resistance of Automotive Coatings 405 Gerhard Pausch and J¨ rg Schwarz o 12.2.1 Introduction 405 12.2.2 Environmental Impact on Coatings 406 220.127.116.11 Natural Weathering 408 18.104.22.168 Artiﬁcial Weathering 414 22.214.171.124 New Developments 421 12.2.3 Standards for Conducting and Evaluating Weathering Tests 423 12.2.4 Correlation Between Artiﬁcial and Natural Weathering Results 426 12.3 Corrosion Protection 427 Hans-Joachim Streitberger 12.3.1 Introduction 427 12.3.2 General Tests for Surface Protection 429 12.3.3 Special Tests for Edge Protection, Contact Corrosion, and Inner Part Protection 432 12.3.4 Total Body Testing in Proving Grounds 433 12.4 Mechanical Properties 434 Gerhard Wagner 12.4.1 General Remarks 434 12.4.2 Hardness 435 126.96.36.199 Pendulum Damping 435 188.8.131.52 Indentation Hardness 436 184.108.40.206 Scratch Hardness 439 12.4.3 Adhesion and Flexibility 441 220.127.116.11 Pull-Off Testing 441 18.104.22.168 Cross Cut 441 22.214.171.124 Steam Jet 444 126.96.36.199 Bending 445 188.8.131.52 Cupping 446 184.108.40.206 Impact Testing by Falling Weight 448 12.4.4 Stone-Chip Resistance 449 220.127.116.11 Standardized Multi-Impact Test Methods 450 18.104.22.168 Single-Impact Test Methods 451 12.4.5 Abrasion 454
Contents XV22.214.171.124 Taber Abraser 454126.96.36.199 Abrasion Test by Falling Abrasive Sand 45512.4.6 Scratch Resistance 456188.8.131.52 Crockmeter Test 456184.108.40.206 Wet-Scrub Abrasion Test 457220.127.116.11 Simulation of Car Wash 45818.104.22.168 Nanoscratch Test 46012.4.7 Bibliography, Standards 46213 Supply Concepts 467 Hans-Joachim Streitberger and Karl-Friedrich D¨ ssel o13.1 Quality Assurance (QA) 46713.2 Supply Chain 46813.2.1 Basic Concepts and Realizations 46813.2.2 Requirements and Limitations of a System Supply Concept 47314 Outlook 475 Hans-Joachim Streitberger and Karl-Friedrich D¨ ssel o14.1 Status and Public Awareness of the Automotive Coating Process 47514.2 Regulatory Trends 47614.3 Customer Expectations 47814.4 Innovative Equipments and Processes 47914.5 New Business Ideas 481 Index 483
XVIIPrefaceIt is now over 10 years since the ﬁrst publication of ‘‘Automotive Paints andCoatings’’ in 1996. The original publication was made possible thanks to theuntiring effort of Gordon Fettis to bring out a book dedicated to automotiveOEM coatings. In a changing business environment, the automotive industry isalways reevaluating its core competencies and has transferred many technicaldevelopments and manufacturing tasks to the supplier industry. Painting, so far,has remained one of its core competencies and is a ‘‘value added’’ process inthe car manufacturing industry. This fact underlines the necessity for a new andcompletely revised edition of the book. We thank Mr. Fettis for taking this up, andgiving us the opportunity to publish this book. We also thank all the contributors fortheir articles that demonstrate the expertise of each of them in his respective ﬁeld. The book covers the painting process of passenger cars and ‘‘light trucks’’, asthey are called by the American automotive industry. These vehicles are massmanufactured and therefore their coating requirements in terms of processing andcoating performance are similar in nature. The key performance drivers in automotive coatings are quality, cost, andenvironmental compliance. Quality, in this context, relates to corrosion protectionand long lasting appearance. Quality and cost are addressed by more efﬁcientcoating processes and a higher degree of automatization. This has led to reduceduse of paint and lesser waste per body. With the widespread use of high solid,waterborne, and powder coatings, solvent emission from paint shops have beenreduced by more than 50% over the last ten years. We are proud to contribute to this development by publishing the second editionof ‘‘Automotive Paints and Coatings’’, in which we try to describe the state-of-the-arttechnology of automotive coating processes and the paint materials used in theseprocesses. Automotive coating processes represent the cutting edge of application tech-nology and paint formulations. They are the most advanced processes in regardto volume handling, sophisticated body geometries and speed in mass produc-tion. Colored coatings offer mass customization and product differentiation at anaffordable cost.Automotive Paints and Coatings. Edited by H.-J. Streitberger and K.-F. D¨ ssel oCopyright 2008 WILEY-VCH Verlag GmbH & Co. KGaA, WeinheimISBN: 978-3-527-30971-9
XVIII Preface This second edition may help many readers to understand these high-performance coating processes and the related materials, and also appreciate the scope for new ideas and innovations. The contents and the main focus of this edition differ from those in the ﬁrst edition. Processes, technology, and paint formulations have been weighted equally, reﬂecting that legislation and cost were the driving forces of the past. We hope that not only experts but also technically interested readers will ﬁnd this book useful. M¨ nster and Wuppertal, Germany u Dr. Hans-Joachim Streitberger December 2007 Dr. Karl-Friedrich D¨ssel o
XIXAbbreviations1K 1-component2K 2-componentABS Acrylonitrile-Butadiene-StyreneAED Anodic Electro DepositionAFM Atomic Force MicroscopyAPEO AlkylPhenolEthOxylateASTM American Society for Testing and MaterialsATRP Atom Transfer Radical PolymerizationBAT Best Available TechnologyBSC Balanced Score CardBMC Blow Molding CompoundBPA BisPhenol-ACASS Copper Accelerated Salt Spray testCCT Cyclic Corrosion TestCED Cathodic Electro DepositionCIE Comite International d’EclairageCMC Critical Micelle ConcentrationCPO Chlorinated PolyOleﬁnesCPU Cost Per UnitCSM Centre Suisse d’electronique et de MicrotechniqueCTE Coefﬁcient of Thermic ExtensionDBP Di-ButylPhtalatDDDA DoDecane-Di-AcidDDF Digital Dichtstrom F¨ rderung (digital dense ﬂow transporation) oDIN Deutsche IndustrieNorm (German industrial normation ofﬁce)DMPA DiMethylol-Propronic AcidDOI Distinctness Of ImageDOS DiOctylSebacateDPE DiPhenylEthaneEDT Electro Discharge TexturingEDTA Ethylene Diamino Tetra AcidEEVC European Enhanced Vehicle safety CommitteeAutomotive Paints and Coatings. Edited by H.-J. Streitberger and K.-F. D¨ ssel oCopyright 2008 WILEY-VCH Verlag GmbH & Co. KGaA, WeinheimISBN: 978-3-527-30971-9
XX Abbreviations EINECS European Inventory of Existing commercial Chemical Substances EIS Electrochemical Impedance Spectroscopy EN European Norms EO EthOxy EP EPoxy EPA Environmental Protection Agency EPDM Ethylene-Propylene-Diene-Monomer ERP Enterprise Resource Planning ESCA Electron Spectroscopy for Chemical Analysis ESTA ElectroSTatic Application FEM Finite Element Method FMVSS Federal Motor Vehicle Safety Standards (USA) GMA GlycidylMethAcrylat HALS Hindered Amine Light Stabilizer HAPS Hazardous Air Polluting Substances HDI 1.6-HexamethyleneDiIsocanate HDI HexamethyleneDiIsocanate HLB Hydrophilic Lipophilic Balance HMMM HexaMethoxyMethylMelamine HVLP High Volume Low Pressure ICEA IsoCyanatoEthyl(meth)Acrylate IPDI IsoPhoronDiIsocyanate IPN InterPenetrating Network IPP Integrated Paint Process ISO International Standard Organisation KPI Key Performance Indicator LEPC Low Emission Paint Consortium MCC Mercedes Compact Car MDI Diphenyl-Methan-DiIsocyanate MDF Medium Density Fibreboard NMMO N-MethylMorpholine-n-Oxid NAFTA NorthAmerican Free Trade Agreement NTA NitroloTriAceticacid OEM Original Equipment Manufacturer PA PolyAmide PA-GF Glas Fiber reinforced PolyAmide PBT PolyButyleneterephtalate PC PolyCarbonate PFO Paint Facility Ownership PMMA PolymethylmethAcrylate PO ProprOxy PP PolyPropylene PPE Poly Phenylene Ether PUR PolyURethane
Abbreviations XXIPVC PolyVinylChlorideQC Quality ControlQA Quality AssuranceQUV Tradename for test chambers (Q-Lab)RAFT Reversible Addition Fragmentation chain TransferRCA Rheology Contol AgentRRIM Reinforced Rejection InMoldRT Room TemperatureR-TPU Reinforced ThermoPlastic PolyurethaneSAE Society of Automotive Engineers (USA)SCA Sag Control AgentSCM Supply Chain ManagementSDAT Short safe Drive Away TimeSEA South East AsiaSMC Sheet Molding CompoundSNIBS Sodium NItroBenzeneSulfonateTACT Tris(AlkoxyCarbonylamino)-1.3.5-TriazineTDI Toluylene DiIsocaynateTEM Transmission Electron MicroscopyTEMPO TEtraMethylPiperidin-n-OxidTGIC TriGlycidylIsoCyanuratm-TMI 3-isoporpenyl-dimethylbenzyl-isocyanateTMXDI Tetra-Methyl-Xylylene-DiIsocyanateToF-SIMS Time of Flight Secondary Ion Mass SpectroscopyTPO ThermoPlastic OleﬁnesUP Unsaturated PolyesterUV UltraVioletteUVA UV-AbsorberVDA Verband der Deutschen Automobilindustrie (German association of car manufactureres)VOC Volatile Organic Compounds
XXIIIList of ContributorsBernd Burchardt Gabi Kiegle-B¨ckler oSika Schweiz AG BYK-Gardner GmbHOEM Adhesives & Sealants Lausitzerstr. 8T¨ ffenwies 16 u 82538 Geretsried8048 Z¨ rich u GermanySwitzerland Peter W. Merz Sika Schweiz AGKarl-Friedrich D¨ssel o OEM Adhesives & SealantsDupont Performance Coatings T¨ ffenwies 16 uChristbusch 25 8048 Z¨ rich u42285 Wuppertal SwitzerlandGermany Gerhard PauschHorst Gehmecker Pausch Messtechnik GmbHChemetall GmbH Nordstr. 53Trakehnerstr. 3 42781 Haan60407 Frankfurt GermanyGermany Heinz-Peter Rink BASF Coatings AGStefan Jacob CTS Trailers, Trucks & ACEMankiewicz Gebr. & Co. Automotive Reﬁnish / CommercialGeorg-Wilhelm-Str. 189 Transport Coatings Solutions21107 Hamburg Glasuritstr. 1Germany 48165 M¨ nster-Hiltrup u GermanyDobrivoje JovanovicSika Schweiz AG J¨rg Schwarz oOEM Adhesives & Sealants Daimler AGT¨ ffenwies 16 u Werk Sindelﬁngen – B 430 – PWT/VBT8048 Z¨ rich u 71059 SindelﬁngenSwitzerland GermanyAutomotive Paints and Coatings. Edited by H.-J. Streitberger and K.-F. D¨ ssel oCopyright 2008 WILEY-VCH Verlag GmbH & Co. KGaA, WeinheimISBN: 978-3-527-30971-9
XXIV List of Contributors Hans-Joachim Streitberger Gerhard Wagner Markt & Management Dupont Performance Coatings Patronatsstr. 13 Qualit¨tspr¨ fung a u 48165 M¨ nster u Christbusch 25 Germany 42285 Wuppertal Germany Pavel Svejda D¨ rr Systems GmbH u Guido Wilke Application Technology Hochschule Esslingen Vertrieb/Sales University of Applied Sciences Rosenstr. 39 Labor Polymerwerkstoffe 74321 Bietigheim-Bissingen Kanalstr. 33 Germany 73728 Esslingen Germany Klaus Werner Thomer Adam Opel AG Heinrich Wonnemann ITDC/ME BASF Coatings AG Friedrich-Lutzmann-Ring CO/XEH – B325 65423 R¨ sselsheim u 48165 M¨ nster u Germany Germany
11IntroductionHans-Joachim Streitberger1.1Historic DevelopmentThe car painting industry has undergone incredible changes by way of materials andprocesses development following the general progress of manufacturing technologyfrom the start of the twentieth century until today. Early coating processes, that is,during the ﬁrst half of the twentieth century, involved the use of air drying paints,sanding of each layer and polishing, all of which needed weeks for completion. Allthe coating steps were executed manually (Figure 1.1). Different driving forces behind the development of better and more efﬁcientprocesses have brought in dramatic changes over the last 100 years. Introduction ofmass production requiring faster curing paints, better ﬁlm performance in termsof corrosion and durability of colors, improved environmental compatibility, andfully automated processes for better reliability characterize the most importantmilestones in this ﬁeld (Table 1.1). The status of mass production of cars during the 1940s required new coatingsproviding faster drying and curing: the result – the birth of enamels! At the sametime, owing to their limited availability, the natural raw materials used in themanufacture of the paints had to give way to synthetic chemicals. Crosslinkingof paints became state of the art. The coating process could be reduced to a dayincluding all necessary preparation time for the car body like cleaning, sanding,repairing, and so on. The number of applied coatings had been reduced to four or ﬁve layers, all handsprayed this time (Figure 1.2). The function of these layers were corrosion protec-tion for the primers, smoothness and chip resistance for the primer surfacers (whichare often applied at the front ends and exposed areas in two layers), and color andweather resistance for the ﬁnal top-coat layer. In the 1950s the process of applyingthe primer changed to dip coating, a more automated process, but a hazardousone owing to the solvent emission of the solvent-borne paints. Explosions andﬁre hazards then forced automotive manufacturers to introduce either waterbornepaints or electrodeposition paints. The latter, which were introduced during theAutomotive Paints and Coatings. Edited by H.-J. Streitberger and K.-F. D¨ ssel oCopyright 2008 WILEY-VCH Verlag GmbH & Co. KGaA, WeinheimISBN: 978-3-527-30971-9
2 1 Introduction Fig. 1.1 Painting of cars in the 1920s and 1930s. Table 1.1 Milestones and driving forces in the car coating process Year Topics/Driving forces Aspects 1920 Manual painting Time-consuming process : weeks 1940 Mass production Enamels/oven/time : day 1970 Improved ﬁlm performance CED/2-layer top coat/new materials 1980 Environmental compliance Waterborne coatings/powder/transfer efﬁciency 2000 Automated processes First time capability/time : hours 40µm Clear coat 15µm Base coat 30µm Primer surfacer 20µm CED- primer 1µm Pretreatment Substrate Fig. 1.2 Scheme of the multilayer coating of cars.
1.1 Historic Development 3late 1960s, are more efﬁcient in terms of material transfer as well as throwingpower that is necessary for improved corrosion protection of the inner parts of thecar body. In the 1970s the anodic deposition coatings, mostly based on maleinizedpolybutadiene resins, quickly gave way to cathodic ones owing to better corrosionprotection by their modiﬁed epoxy resin backbones and reactive polyurethane-basedcrosslinkers, increased throwing power, and higher process reliability. At the sametime, the single layer top coats were gradually replaced by two-layer top coatsconsisting of a thin base coat and a thicker clear coat applied wet-on-wet. The basecoats are responsible for color and special effects (for example, metallic ﬁnish),whereas the clear coats provide improved durability using specially designed resinsand formula ingredients like UV-absorber and radical scavengers. Today, mostclear coats in Europe are based on two-component (2K-) formulation consisting ofan acrylic resin with OH-functions and a reactive polyurethane crosslinker. Therest of the world still prefers the one-component technology based on acrylic resinsand melamine crosslinkers. An interesting one-component technology based oncarbamate functionality has been recently introduced in the United States . All these developments contributed to an improved ﬁlm performance resultingin better corrosion protection and longer top-coat durability – for example, glossretention for up to 5–7 years was observed in Florida. Furthermore, raw material development in the pigment section, with improvedﬂake pigments based on aluminum and new interference pigments that changecolor depending on the angle in which they are viewed, has resulted in enhancedbrilliance and color effects of automotive coatings . Along with this development of coating and paint technology, spray applicationtechniques also underwent signiﬁcant improvements. Starting with simple pneu-matic guns and pressure pots for paint supply, today, craftsmanship in painting isno longer needed. Several factors have contributed to the development of coatingmachines and robots and the state of automation that is present today. The ﬁrstfactor was the health risk to the painters who were exposed to solvent emissionfrom paints in the spray booth and the investment in safety equipment, which wasoften unsuitable for them. The second factor was the hazards of the electrostaticapplication technique. Yet another factor was the lack of uniform quality in amanual painting job. Because of the latest developments in wet-on-wet coating technology, coatingmachines, automated cleaning processes, and modern paints, the time taken todayfor the coating process, including pretreatment, can be as short as 8 hours for a carbody leaving the body shop and entering the assembly line (Figure 1.3) . Together with the continuous improvements of the application technology, newwater-based materials were developed to contribute toward the legally enforcedenvironmental compliance of the processes. The ﬁrst water-based base coats wereintroduced at Opel in Germany in the 1980s, followed by water-based primersurfacers in the 1990s. Investments in modern paint shops vary from ¤200 up to ¤600 million for coat-ing 1000 units a day. Today, painting technology for the car industry has been more
4 1 Introduction Body-in-white Washer Pretreatment CED Baking oven Drying Sound Sealing Sanding dampers Cleaning Primer surfacer application Baking oven Baking oven Clear coat Flash off Basecoat Cleaning Inspection Repair Waxing To Assembly line Back to “Cleaning” before Spotrepair primer surfacer application Fig. 1.3 Process steps in modern automotive paint shops. or less standardized all over the world. Inorganic pretreatment, cathodic electrode- position, liquid or powder primer surfacer, liquid base coats, and one-component or two-component solvent-borne clear coats are mostly used today. This is a result of the consolidation of the engineering and coating line manufacturers and paint producers into just a handful of major players. In 2002, 70% of the car coating market was in the hands of Dupont, PPG, and BASF. As of today, the technology of powder coatings has reached a point where many car manufacturers have decided to introduce environmentally compliant technology more aggressively. Today, powder is established as the primer surfacer in North America: at Chrylser in all actual running plants, at GM for their truck plants, and in all new paint shops. In Europe, in a number of plants at BMW, powder is also used as a clear coat. . Over the same period of time, body construction materials have also changed signiﬁcantly. Starting with pure steel bodies, today the share of aluminum and magnesium, as well as plastic, as raw materials for speciﬁc car components or hang-on parts can account for about 30% of the weight of the car. On an average, half of this is plastic. The main focus is on weight reduction, design variability, and cost (Figure 1.4). Starting with bumpers in the 1970s, and moving on to fenders and hoods, many of the exterior parts are now made of specially designed plastics. The coating process is predominantly outsourced for these parts, even though some car manufacturers assemble the parts in the coating line and apply the original base coat–clear coat technology on these parts to overcome color match problems.
1.1 Historic Development 5 Glass 3.3 Rubber 5.0 Plastics 8.6 Steel 60.7 Zinc 0.4Copper/Brass 1.6 Al 8.7 Iron 11.8Fig. 1.4 Share (%) of different material classes for carmanufacturing (source : Ward’s Communications, Facts &Figures 2002). Interior parts made of plastic materials were introduced in the 1960s and aretoday increasingly being coated by specially formulated paints for providing the ‘softfeel’ touch that gives the plastic an improved acceptance by the customers. Theseparts were mostly painted by the part manufacturers and supplied to the automotiveindustry as complete modules to the assembly line. Special laser coatings havebeen developed to inscribe symbols of functions on coated dash board or otherunits in the interior of a car. Another increasing application of coatings is connected with the modern designof head lamps made of blow molding compounds(BMC) for the head lamp reﬂectorscovered by a polycarbonate lens. Both parts are coated dominantly by UV coatings. Many other exterior parts like hoods and trunk lids, as well as other bodysegments, are increasingly made of aluminum or sheet molding compounds(SMC). In addition to the aspect of careful construction in respect of buildinggalvanic elements, pretreatment chemicals and the process of multimetal bodieshad to be developed. This was a demanding task that needed avoidance of anyharmful heavy metal ions like chromic-VI. The complete aluminum body stillremains a niche product. Connected with an increased share of multicomponent parts of different sub-strates, the welding process for manufacturing cars has been partially replaced byother assembling techniques like clinching and riveting. Glewing, a technologyknown from the air transportation industry, has become very important. This tech-nique is based on surface treatment and product application similar to coatings.On the basis of the use of interface with coating layers like gluing back-windowson electrocoat layers and its increasing application, this will be described inChapter 10. The performance requirements for an OEM (Original Equipment Manufacturer)coating of passenger cars are many and diverse. They can be attributed to corrosionprotection, durability, including stone chip resistance, and appearance. One shouldbear in mind the extent of extreme stress that cars are exposed to throughouttheir life span. High temperatures up to 70 ◦ C on dark colors in Florida andsimilar regions, as well as low temperatures of –50 ◦ C in polar regions, permanent
6 1 Introduction temperature ﬂuctuation of 10–20◦ C daily, stone chip attacks on unpaved roads, high loads of salt in coastal regions, as well as in wintertime, high ultraviolet radiation in combination with dry and humid periods, the action of acid or alkaline air pollutants from many sources, and the physical and mechanical stress in vehicle washing installations are the most important among the many factors. Recently, the gloss, appearance, and effect coatings became important factors for selling cars by underlining the image and personality of the car and its driver. Because of the fact that many resources have been directed to the environmental improvement of paint application as well as toxic aspects of the paint formulas, the performance of automotive coatings has increased signiﬁcantly. Even the ﬁlm thickness of a car coating today is only 100–140 µm, which needs, in most coating processes, about 9–16 Kg deposited paint per car; the corrosion protection and the long time durability of color and gloss is about two times higher than what it was 25 years ago. Three main factors have contributed to this: new substrates, introduction of cathodic electrodeposition paints, and the two-layer top-coat system with a special designed clear coat for long term durability. The life time of a car is no longer related to the corrosion or durability of the coating and color. The color of cars has become a very important design tool, signiﬁcantly support- ing the purchasing habits of customers. For this reason, color trends are being observed by the paint and automotive industry together to develop trendy colors for the right cars. The color variability has been increased at the same time. Today’s customers, es- pecially in the premium car level, can demand whichever colors they want at a cost. New color effects like ‘color ﬂop’, which is a coating providing different color impres- sions to the customer depending on the angle of vision, have entered the scene . The latest signiﬁcant milestone in the history of the development of car painting is the combination of highly efﬁcient application techniques like high rotational mini- or micro-bells and the painting robots (Figure 1.5). This has lead to the highest degree of transfer efﬁciency and reliability, resulting in an efﬁciency of 90% and more of defect free coatings in modern paint shops . The application of sealants, sound deadeners and underbody protection is very often a part of the coating process. These materials need to be dried. In an efﬁciency move, the primer baking ovens are mostly used for this process. Shorter cycle time of car models requires faster planning and realization periods for designing new paint shops. Additionally, globally competitive business has brought into the focus of car manufacturers not only the respective investment costs, but also the running cost of a coating line . At the end of the paint line, the application of transport coatings, wrap up of coated cars for company design on a commercial ﬂeet, as well as safety measures, all become part of the coating processes connected with the manufacture of cars . Quality assurance has reached a new dimension for automotive OEM paints and coatings. While time-consuming batch-to-batch approvals of the customer’s speciﬁcations has been the order of the day, supporting-system approaches, for example, audit-management systems according to DIN-ISO 9001 and 14001, ISO/TS 16949, QS 9000 or VDA 6.1, have become mandatory for the paint industry
1.2 Legislation 7Fig. 1.5 Paint robot with electrostatic bell (source: BASF Coatings).to be approved as a supplier to the automotive industry. So, right from thebeginning, the development of new products has to be quality oriented to ‘zerodefect’ levels through all the steps leading up to the delivery status. At the same time, the testing and physical methods of describing the performanceof paint and coatings have become much more precise and value based not onlyfor the performance of the ﬁlms, but also the performance during the applicationand ﬁlm forming processes. In top-coat color speciﬁcations and in general physicalcolor matching, especially, colorimetric data will replace visual inspections, whichhave reliability problems. The so-called ‘ﬁnger print’ methods have been developedto improve the performance of paints during the application processes . Filmperformances like durability and corrosion protection, and mechanical performancelike scratch, mar, and gravel resistance are very predictable in short term testingprocedures today.1.2LegislationAnother driving force for ﬁnding new coating formulas is the passing of legislativeacts all over the world calling for a ban on toxic components in all the formulae
8 1 Introduction to the maximum possible extent . So lead- and chrome-free paint formulas are today ‘state of the art’. Also, the emission of volatile organic compounds (VOC) has been restricted, especially in Europe and the NAFTA (North American Free Trade Agreement) region for the last 20 years, to numbers that are deﬁned in various ways and controlled in NAFTA and Europe, and are about ﬁve to ten times lower than what they were 30 years ago. This was reached by simultaneous material and process development as described herein. The industry has to deal with moving targets set by the authorities according to the best available technology. In general, the emission of any type of ‘greenhouse gases’ is in worldwide focus based on the ‘Kyoto’ protocol. Life cycle assessments are gaining awareness . Owing to the fact that the most important application processes of automotive paints release solvents and that the composition of coatings can have more than 15 ingredients, together with the global agreements on environmental targets, the political scenario in North America and Europe was to focus ﬁrst on paint consumers and manufacturers for improved environmentally compatible products and application processes. The response in the 1980s in North America was to increase the solid contents and decrease the solvents of the actual solvent-borne paint formulations. New resins had to be developed and formulation as well as application conditions had to be optimized in the direction of sagging resistance and surface and ﬁlm properties. The relative increase of solids by about 20% generated a completely new technology. The legislation controlled the progress by measuring the solvent input in the factories. In Europe the resources for research and development were directed to waterborne coatings ﬁrst, resulting in the introduction of waterborne base coats. Solvent-borne base coats were the paints providing the highest amount of solvent emission owing to the very low solid content of 12–18% at that time. Later in the 1990s waterborne primer surfacer and some waterborne clear coats were in- troduced. The legislation in Germany supported abatement technology to meet its requirements. The new European approach of the VOC directive of 1999 now combines after-treatment with the pragmatic approach of North America, mostly the United States. Both paint development directions resulted in rather different paint formulations, creating problems for the South East Asia (SEA) region, which still has to decide which way to go. Signals and recent decisions of Toyota, Honda, Nissan, and Mitsubishi favor the waterborne products. Safety standards for the handling of paints in the paint kitchen as well as application booths are quite uniform around the world. The personal safety equipment in spray booths now mostly consists of complete overall, mask, and respiratory systems protecting the worker from any contamination. A greater use of robots keeps workers out of the paint booth. They become engineers who program and run the robots and look into other booth parameters. Harmful chemicals and additives have been tested comprehensively during the last 30 years. Many products have been abandoned either by the car manufacturers themselves or by legislation. Among these are lead, in electrocoatings and pigments,
1.3 Automotive and Automotive Paint Market 9chromium, in primers and electrocoatings, cadmium, in pigments, many solventsqualiﬁed as HAPS (Hazardous Air Polluting Substances), and monomers likeacrylonitrile, acrylamide, and so on, which belong to the cmr (carcinogenic,mutagenic, reproduction toxic) products. Special awareness has been created withrespect to the biozides in Europe . Other VOCs may contribute to the generationof ozone in the lower atmosphere and so they have been limited by legislation, stepby step, leading up to the best state-of-the-art technology of the paint applicationprocess  as well as paint product development. Signiﬁcant steps have been madein this respect by the introduction of waterborne base coats, waterborne primer,and the slurry-clear coat. Further reduction in VOC can be achieved by powderprimer surface and powder clear coat . In recent years, legislation in Europe focuses on the harmful and environmentallysigniﬁcant impact of chemicals. This will also lead to further replacement ofingredients and components in paint formulation .1.3Automotive and Automotive Paint MarketIn 2004, car manufacturers, worldwide, produced about 58 million cars and lighttrucks (vans, mini-vans, pickups). Europe, North America, and Japan are tradition-ally the largest producing regions, accounting for about 78% of all cars (Figure 1.6). SEA including Korea, China, and India, is gaining importance as a consumermarket as well as a producing region. This is a change from the past and willchange in the future owing to two main reasons: 1. Today’s quality concepts in manufacturing as well as painting cars allow car manufacturers to produce wherever workforce is available. This drives most of them to regions with low labor costs. 2. Most car manufacturers produce world class cars, which can be exported and brought into all market places around the world. South 58 Mio cars and trucks America Others SEA 4% 4% Europe 14% 34%Japan 11% Nafta 33%Fig. 1.6 Contribution of the regions to world light vehiclecar manufacturing (Automobilprod.Juni/2004).
10 1 Introduction 24.8 Mio t General industry 29% Automotive OEM Architectural 4% 60% Refinishing 3% Printing inks 4% Fig. 1.7 Volume of the worldwide paint market as of 2002. Among the limiting factors are the supply bases of components and hang-on parts, especially when it comes to just-in-time deliveries. This leads to certain regions where the car manufacturers would prefer to settle in the future like North Carolina, South Korea, Eastern Europe, and Shanghai, for example. Since the 1980s, the outsourcing of manufacturing components and integrated modules like headlamps, fenders, bumpers, doors, and roof elements for direct de- livery to the assembly line represents the global trend in worldwide car manufactur- ing so that the ‘value added’ is transferred to the automotive supplier industry. Since 2000, the supplier industry, which has a 40% share of the worldwide production value in the car industry and which includes more of design work, is increasingly focusing on innovation efforts and is consolidating to become a global industry. The worldwide market volume of car paints of about 1.0 Mio t consists of electrodeposition coatings, primer surfacers, base coats, and clear coats, as well as speciality coatings consumed in the automotive coating lines and in the supplier industry, only counts for about 4% of the total paint market (see Figure 1.7). The biggest share contributes to the architectural market, followed by general industry (OEM market), which, in other statistics, like in North America, includes the contribution of car paints. From a technological standpoint, car paints as well as their coating processes are valued as the most advanced technologies both by coating performance, and the efﬁciency and reliability of the coating process. These high standards and requirements forced many players out of business, resulting in the fact that today just three main paint suppliers dominate the worldwide automotive OEM paint market. Regional paint manufacturers exist mostly in Japan and SEA. In recent years, the method of conducting business activities has begun to change signiﬁcantly. With the ‘single sourcing’ concept in which one paint supplier delivers all products and takes responsibility for all paint-related problems of the coating process, the business arrangements between paint manufacturers and the automotive industry has reached a point where the responsibility of running paint lines as well as cost targets have been taken over by the paint supplier . The so-called Tier 1’ suppliers manage the various degrees and levels of cooperation with
1.3 Automotive and Automotive Paint Market 11 500 g m−2 VOC emission 400 300 200 100 0 1975 1985 1995 2005 YearFig. 1.8 Reduction potential of volatile organic compound(VOC) emission of the automotive coating process in gramper square meter body surface based on paint and processdevelopment (best available technology).the customer. Tier 2 suppliers manage the total paint shops including engineering,logistics, auxiliaries, quality control, and stafﬁng . Targeting the cost per unit and not cost per paint, together with new processes, modern application techniques, and paint formulations has brought theefﬁciency and environmental compliance of the coating processes in terms of VOCto a level that could not have been imagined 30 years ago (Figure 1.8). This hashappened with an increased performance level of coatings in terms of corrosionprotection, the top coat’s long-term durability in respect to chip resistance, andcolor and gloss retention.References 1 Green, M.L. (2001) Journal of Coat- 11 Papasauva, S., Kia, S., Claya, J., ings Technology, 73 (981), 55. G¨ nther, R., (2002), Journal of Coat- u 2 Rochard, S. (2001) Modern Paint ings Technology, 74 (925), 65. and Coatings, 91 (9), 28. 12 Hagerty, B. (2002) Polymers Paint 3 Anonymous, Automobilproduktion Colour Journal, 192 (4451), 13. (12/2000) 38. 13 Drexler, H.J., Snell, J. (04/2002) 4 K¨ nneke, E. (2002) Journal f¨ r o u Oberﬂ¨ chentechnik, 42 (3), 64. a European Coatings Journal, 24. 5 Cramer, W.R., Gabel, P.W. 14 Klemm, S., Svejda, P. (2002) Journal (7–8/2001) European Coatings Jour- f¨ r Oberﬂ¨ chentechnik, 42 (9), 18. u a nal, 34. 15 Scott, A. (2007) Chemical Work, 169 6 Hoffmann, A. (2002) Journal f¨ ru (11), 17. Oberﬂ¨ chentechnik, 42 (3), 54. a 16 Esposito, C.C. (2004) Coatings World, 7 Gruschwitz, B. (2004) Metalloberﬂ¨ che a 9 (3), 21. 58 (6), 22. 17 (a) Cramer, W.R. (2005) Fahrz. + 8 Vaughn-Lee, D. (2004) Polymers Paint Kaross., 58 (5), 34. (b) Bloser, F. Colour Journal, 194 (4478), 24. (2004) Coatings Yearbook, Vincentz, 9 Voye, C. (2000) Farbe Lack, 106 (10), 34. Hannover. 10 Shaw, A. (2001) Modern Paint 18 Wegener, E. (2004) Coatings World, 9 and Coatings, 91 (2), 13. (10), 44.
132Materials and Concepts in Body ConstructionKlaus Werner Thomer2.1IntroductionFrom the days of the carriage to the efﬁcient car bodies of today, in the courseof over 120 years, the automotive industry has undergone enormous changes.Technological progress, the use of new and better materials, the basic conditions oftransportation and the politics surrounding it, as well as general, social, and culturalchanges have all, more or less, contributed to the evolution of the automobile towhat it is today (Figure 2.1). Whereas, in the beginning, bodies were built on frames, today the body frameintegral (BFI) or self-supporting body is used in the manufacture of passengercars. The body on frame (BOF) mode of construction is used only for trucks andoff-road vehicles. The BFI is a complex way of construction, with a large number ofrequirements to be met. All parts of a car are attached to the body, which constitutesthe core carrier and is called the body-in-white. Design, space conditions, occupantprotection, and crash performance are important criteria for the customer to makethe purchase decision. To summarize, the body structure fulﬁlls the followingfunctions: • It meets all the structural requirements for all static and dynamic forces. • It provides a crash resistant passenger compartment. • It provides peripheral energy conversion areas. • It provides the platform to mount all drive units and the axle modules. In addition, there are other requirements to be met during the body manufac-ture, for example, part forming, assembly sequence, use of existing manufacturingequipment, low part proliferation, optimized material utilization, design of parts,body-in-white coating, modular method of construction, dimensional accuracy, andlow production cost (Table 2.1, Figure 2.2) [1, 2].Automotive Paints and Coatings. Edited by H.-J. Streitberger and K.-F. D¨ ssel oCopyright 2008 WILEY-VCH Verlag GmbH & Co. KGaA, WeinheimISBN: 978-3-527-30971-9
14 2 Materials and Concepts in Body Construction Lancia Lambda Pressed steel Large scale presses Fully galvanized Aluminum — space frames for steel sheets steel body frame Carriage Line assembly Self-supporting Higher strength manufacturing body thin steel sheets Source: ThyssenKrupp steel AG Fig. 2.1 Milestones in car body manufacturing. Table 2.1 Materials and Manufacturing Methods for Advanced Car Body Design Materials Manufacturing Methods High-strength steel Tailored blanks Aluminum Hydroforming Magnesium Coated blanks Plastics Saving of process steps (Pretreatment, FRP: Fibrous glass reinforced plastics posttreatment, prepunching,. . .) CFRP: Carbon-ﬁber reinforced plastics Complex, large light-weight metal Composite sheets (sandwich, foam, . . .) castings Material mixture Deep drawing and simultaneous attachment of fasteners Combination of functions (joining and attaching) Hybrid joining (mechanical joining and bonding) Advanced car body design The speciﬁcations for a certain body type cover hundreds of details and parameters that can increasingly be handled only by computerization. The demand for shorter development periods, starting with the original idea, covering design concepts, and up to development of prototypes and saleable cars, can safely be realized only by using analytical methods.
2.2 Methods of Body Construction 15Source: Porsche AGFig. 2.2 Evaluation in car body manufacturing.2.2Methods of Body ConstructionIn principle, a distinction can be made among various types of body construction.The most common form is the monocoque design. In the last few years, newdevelopments have emerged in this ﬁeld, among which the space-frame conceptis of great importance. There are some hybrid forms also, which combine bothmethods of construction.2.2.1Monocoque DesignIn the construction of self-supporting bodies, steel bodies have been used aboveall others, in the monocoque design (Figure 2.3). Here, formed sheet-metal panelsare joined, preferably by weld spots. The body-in-white consists of the underbodyassembly made up of the front compartment, the center ﬂoor and the rearcompartment. In addition, there are the side panels, which together with theunderbody assembly and the roof, form the box-type body-in-white. The add-onparts like doors, trunk lid, and fenders complement the body-in-white . The lower part of the underbody is formed by longitudinal and cross members.At the front and the rear ends, these are terminated by ﬂoor panels. The twolongitudinal front members, which are made of the longitudinal front and itsextension, are provided with a closing plate at the front end, on which the bumperis fastened. For the remaining longitudinal members, locators are welded at thelower side to position the chassis member. In addition, the engine mounts areaccommodated on these front longitudinal members. The front frame, which takesthe engine and the front axle, also plays a major role as an energy-absorbingcomponent during a frontal crash, and is reinforced at the points with the highestload impact. In most cases, the extension of the front frame ends at the connection
16 2 Materials and Concepts in Body Construction Front compartment Center floor Rear compartment Underbody assembly Side panels and roof Body in white Fig. 2.3 Monocoque design. of the seat cross member to the ﬂoor panel. The extension primarily serves to avoid a deﬂection of the ﬂoor panel during driving, and in case of a crash. The seat cross member ensures a stiff connection of the front seats. The inner panels needed for the rear underbody are formed by the two longitudinal rear frame members and three cross members for the rear ﬂoor panels, the rear axle, and the back panel. To obtain a better ﬂow of forces, the rear frame is directly connected to the rocker panel, thus increasing the stiffness of the entire body. During driving, the cross member situated at the rear area ensures that the ﬂoor panel in the area of the rear seats does not deﬂect too much. In case of a rear-end impact, it counteracts deformations of the underbody. In addition, the cross member of the rear axle is decisive for the torsional stiffness. Moreover, it stabilizes the rear frame in case of a rear-end crash, and prevents an uncontrolled buckling. As a girder subject to bending, it counteracts strong torsions of the rear frame that may be produced as a result of a counterrotating deformation of the rear frame sections. The back panel cross member serves to prevent deﬂection of the ﬂoor panel in the trunk area. The wheelhouse is welded inside the vertical ﬂange of the rear frame. The reinforcement of the back panel takes up the extensions of the wheelhouse. These extensions are important for the torsional stiffness of the entire body, and the local stiffness of the rear opening. In this manner, an additional load path is created for a rear-end crash. Front parts are attached to the underbody. The upper front part takes up the locking for the hood and the radiator mounting, and the lateral front parts take up the headlamps and the front wheelhouse. The locator of the shock-absorbing strut, which takes up all reaction forces of the strut, is positioned on the wheelhouse. To
2.2 Methods of Body Construction 17achieve sufﬁcient stiffness, the wheelhouse is connected to the front frame througha preferably straight element acting as a tension rod. Above the wheelhouse, thereis a strut, which in case of a frontal crash, induces forces in the A-pillar and the doorwindow channel, before it absorbs energy by a controlled forming process. At therear end, the wheelhouse terminates with the lateral part of the dashboard panel.Cross to it, is the dashboard panel, which together with the closing plate and theextension of the front ﬂoor, separates the engine compartment from the passengercompartment. Furthermore, the closing plate protects the passenger compartmentfrom noise and contamination, and prevents the engine or other components frompenetrating the interior in case of a crash. Dashboard panel penetration after acrash is therefore a measure of the structural quality of the body, and it is oftenused for comparison. Above the dashboard panel there is a reinforced cover, whichforms the windshield opening together with the inner A-pillar and the front roofframe. The side panel assembly essentially consists of an inner and an outer part.In the door opening area, these two shells form the pillar cross sections togetherwith the inner A-pillar. For many cars, the A-pillar cross sections include additionalreinforcements. In the case of convertibles, some of these reinforcements aremade of high-strength pipe cross sections or hydroformed parts. The B-pillar crosssection is provided with door weather strips on both sides. In addition, the B-pillaraccommodates the hinges for the rear door with further local reinforcements.These reinforcements also serve to acoustically reduce diagonal deformations inthe door openings during normal driving. Moreover, the reinforcement of theB-pillar is important during a lateral impact because it prevents a penetration intothe passenger compartment. In the rear area, there is an extension at the side panel.An extension piece surrounds the opening for the tail lamps. As in the case of theextension of the wheelhouse, this measure is important to augment the torsionalstiffness and the rear-end diagonal stiffness. The roof consists of the outer panel, which is stabilized by bonded bows, and therear frame. Whereas the roof bows do not inﬂuence the total torsional stiffness ofthe body, the rear roof frame plays an important part. Add-on parts are usually all parts which belong to the car body, but which arenot welded to the body-in-white, that is, doors, lid, fenders, and bumpers. Thedevelopment of the add-on parts is characterized by two approaches: • Modular construction – As a result of outsourcing the development and production, add-on parts are increasingly delivered as complete modules to the production line of the car manufacturer. • Use of light-weight materials – The use of new body materials with a lower speciﬁc weight than steel has begun in large volumes, above all for add-on parts. Today, bumpers and fenders are often made of plastics, and the lid and the hood, of aluminum.
18 2 Materials and Concepts in Body Construction 2.2.2 Space Frame The space-frame concept is based on the skeleton design which has been in use since the beginning of the industrial production of cars. A steel or wood skeleton forms a solid structure onto which the secondary and tertiary body parts are mounted as noncarrying parts by means of different joining methods. In the 1960s, a method of construction known as Superleggera was patented by the Carrozzeria Touring Company. Here, a tubular space frame made of steel was covered with aluminum sheets. This method of construction was used for the construction of small-volume sports cars like the Austin Martin (1960) or the Maserati 3500GT (1957). Today, Morgan, the British company, still uses body skeletons made of wood. In the case of super sports cars (like the Lamborghini), the body skeletons are made of steel. For the manufacture of different wrought products, the light-weight material, aluminum has evident advantages over steel. Extruded aluminum sections and cast parts provide low-cost wrought products that can be combined to create a design suitable for aluminum. The use of these products for the construction of car bodies leads to a new design concept, the Audi space frame (ASF) , illustrated in Figure 2.4. With the optimum design, the framework structure can be distinguished by its high static and dynamic stiffness, combined with high strength. Compared to today’s steel bodies in monocoque design, approximately 40% of the weight can be saved by using this concept. A special feature of the ASF is the mixture of wrought aluminum products made of castings, sections, and sheet-metal parts. These parts form a self-supporting frame structure into which each load-bearing surface has Metal sheet Sections Casting Fig. 2.4 Space-frame concept (Quelle : Audi).
2.2 Methods of Body Construction 19been integrated. A characteristic feature is the very large and complex die-castparts. By ribbing and load-adjusted wall thicknesses, a construction mode whichmeets the requirements of strength and weight can be achieved. The large numberof possibilities in designing cast parts permits a functional integration and thus, areduction of the number of parts as well as joining operations. Functions such asconnections, location of hinges, or bolted connections can be integrated withoutany additional parts or joining operations. Another type of wrought products, inaddition to castings and sheet-metal parts, are extruded sections that are used forthe body structure. By extrusion, these sections are created with a high degree of self stiffness. Anychanges of the wall thickness section or ﬂanges that are required for stiffnessor strength reasons can be realized almost at will. The sheet-metal parts of thestructure are joined to the body by mechanical methods (e.g. riveting/clinching) orthermal joining processes (e.g. laser or laser metal-inert-gas (MIG) hybrid welding). Another interesting aspect in the manufacture of the space frame is the modularway of construction and the associated separate design, try out, and manufactureof single vehicle modules.2.2.3Hybrid Type of ConstructionIn the hybrid type of construction, the monocoque and the space frame concept areapplied in one body structure by integrating cast, extruded, or sheet-metal parts asassembly groups or single components, into the car body structure.2.2.4Modular Way of ConstructionOwing to a steady proliferation, the modular way of construction has gainedin importance in the automotive industry. On the one hand, it is expected thatclear advantages can be achieved by a standardization of assembly groups, andmore important, standardizing the interface between modules. This in turn willshorten the time of development by simultaneous engineering. On the other hand,simultaneous fabrication of parts and assembly groups also leads to a decrease inthe time needed for developing the vehicles. If one considers the many types of variants available in large automotivecompanies, it becomes obvious that there are an almost uncountable numberof possibilities. The deﬁnition of suitable interfaces in the vehicle allows for thepossibility of dividing the assembly groups into various modules. An essentialadvantage of such modules is that the interfaces can be deﬁned independent ofbody styles. This permits a higher output of components. Moreover, the storagecost of style-speciﬁc components can clearly be reduced, and the retooling costsincurred for model changes can be minimized. The modular way of constructionaims at simplifying the body-in-white manufacture by deﬁning modules withcertain interfaces. There are various possibilities. For some time now, almost all
20 2 Materials and Concepts in Body Construction manufacturers have applied the platform strategy. This means that different car styles can be built on one engineering basis. This basis is usually the ﬂoor panel group of the body-in-white, on which the so-called hat, in this case, the rest of the body, is placed. The second possibility refers to the modules themselves. This means that certain parts together form one system. In the automotive industry, this refers to the parts such as fenders or entire units like van modules. Usually, they are added in the ﬁnal assembly stage. The modular way of construction offers more ﬂexibility to car makers. By out- sourcing certain assembly groups, that is, procuring them from external suppliers, modules can be ordered just in time, depending on the receipt of the speciﬁc order. Owing to the modular concept, changes concerning the body structure may need to be carried out, which frequently do not comply with the light-weight idea, for example, a stiff frame structure may need to be created, with deﬁned contact surfaces. On the other hand, the modules offer a large number of possibilities such as the addition of different materials to the basic structure, for example, paneling with plastic components. Moreover, such systems make it easier to try out light-construction variants on derived products before integrating them into high-volume models. 2.3 Principles of Design 2.3.1 Conventional Design The design starts with sheet-metal panels which are formed into carriers and ﬁelds. These are assembled by various joining methods. The sections of the body-in-white that are decisive for the carrying capacity are designed as hollow sections. Reinforcements are achieved by beads, reinforcing sheets, or spatial curved surfaces. On the one hand, these sheet-metal reinforce- ments are required for reasons of stability and acoustics, on the other hand, they are needed for manufacturing reasons, to achieve a constant shape of the single parts before assembling them onto car bodies. Actually, interior passenger space and cargo space play a large role in styling a vehicle. The design is based on the structural draft, where the sheet-metal parts are determined, but at the same time, the assembly of the single elements is to be considered as well. Moreover, the body structure is to be divided into assembly groups. Here, the body shape is determined by the plan of the outer panels. It is made up of the body surface as developed during styling in connection with aerody- namics. But it does not constitute a supporting structure; so the design department ﬁrst determines a supporting structure, taking light-construction principles into consideration.
2.3 Principles of Design 21 To present a simpliﬁed view, a passenger cell is a box that consists of frames andsheet-metal ﬁelds. The front and rear ends consist of girders subject to bendingand sheet-metal ﬁelds. Forces are applied through carriers, which may be designedto be open or closed. Closed carriers are characterized by a considerable torsionalstiffness, in addition to the bending stiffness. The points of energy application aredesigned at the structural nodes. Here, especially, loads are investigated taking intoconsideration their bending, torsion, and crash behavior. Sheet-metal parts are designed according to manufacturing principles. Theassembly should have as few parts as possible. In addition, the parts are to bedivided so that deep drawing or any other type of forming is viable. A carrierstructure is formed by joining the parts. Otherwise, the design is based on thefollowing general principles: • as far as possible a direct application and compensation of forces • realization of the maximum of planar moment of inertia and drag torque • microstructuring • use of the natural supporting effect of a curvature. A special task is to design the nodal points of carrying members. The lateralfaces of carriers are to be continued in the nodal points. It is possible to transfer thetorques and forces properly only in this way. Particular care is needed while dividingthe sheet-metal panels at the nodal points. In addition to the solid connection ofthe compounds, deep drawing requirements are also to be considered. Special care is also required for the bead pattern. The position and the form ofthe beads should not permit any straight line passing through free space becausethe moment of inertia is applied only through the sheet-metal thickness, and sostiffening is not possible. To avoid a high local degree of forming, the run outdimensions of the beads should also be observed. As an alternative to beads,crowning can be incorporated into the sheet-metal ﬁeld. This approach is of specialinterest, especially for the outer panels. Another possible method of reinforcementof the sheet-metal ﬁelds is the addition of bonded reinforcing bars. In the ﬁeld of light construction, there is a constant search for new methods ofreinforcing that do not stiffen the material. An interesting variant is given by holessurrounded by collars. Considering designs of different sheet-metal thicknesses, which frequently isthe case in connection with light constructions, attention must be directed tothe concentration of stress due to different degrees of stiffness, for example, astep must be designed at the transition from a small sheet-metal thickness to alarger one. This is especially critical in the area of the door hinges at the pillars.Here, sheet-metal thicknesses of approximately 1.6 mm coincide with thicknessesof approximately 8 mm, making additional reinforcements necessary. Another aspect to be taken into consideration during the design stage is to takeprecautions for a compensation for tolerances at the assembly.
22 2 Materials and Concepts in Body Construction 2.3.2 Design Under Consideration of Light-Weight Construction The improvement of passive passenger safety is one of the many focuses in de- veloping car bodies. The static and dynamic properties form the basis of crash optimization. In the course of only a few years, the requirements have increased from 48 km h−1 with a 100% overlapping and a rigid barrier (referring to the US standard FMVSS-208) to 64 km h−1 with a 40% overlapping and a deformable bar- rier as a design criterion. Here, the stricter occupant injury criteria are fulﬁlled with a greater distance, and the remaining survival space is further enlarged. Since the beginning of the 1990s, the energy to be absorbed per structural unit with reference to the side of the car has increased by more than 80% and continues to increase. Side crashes, according to the European Enhanced Vehicle Safety Committee (EEVC) with 50 km h−1 with the greater barrier height of 300 mm, and the US Federal Motor Vehicle Safety Standards (FMVSS-214) with the increased Lateral Impact New Car Assessment Program (LINCAP) velocity of 40 mph are the required standards today. In the important market relevant, but not legal tests such as the Euro-New Car Assessment Programme (NCAP) and the US Insurance Institute for Highway Safety (IIHS), similar conﬁgurations and speeds are used, although different criteria are applied to the evaluations. As a consequence of these different requirements, especially for side impact, global car manufacturers are faced with great challenges. In the last 20 years, increasing the passive safety was the eminent, driving factor for the body-in-white. The aim is to destroy as much energy as possible during a crash by changing the structural form. As aluminum has a lower strength and less elongation at fracture compared to steel, it can transform less energy by changing form, and the compensation is achieved by means of crash boxes. Given the same build conditions, a steel structure is more favorable in relation to a minimum-occupant load. For designing bodies from the view point of crash relevance, the design of the load paths is very important, especially with reference to front and side crashes, because it determines the course of the carriers and the nodal points. In the case of a front crash, the load is mainly applied over the front longitudinal members and the subframe to the lower vehicle structure situated behind them. The forces are distributed through the front-end cross member as a supporting element of the passenger cell, and through the central longitudinal member, which in turn applies the load onto the ﬂoor structure, the lower nodal points of the B-pillar, and the rocker panel. The crash load is introduced through the connection of the front longitudinal member to the lower roof frame, the so-called A-pillar member, into the upper load path. In the case of a side crash, the rocker panel and the B-pillar transfer the energy. Here, the lateral impact beams located in the door are the most important connection for transfer of the load onto the A-pillar and the B-pillar. Today, in addition to safety, another question that is asked in car building, is the one about light-construction aspects. In relation to the design, this means basic changes in the selection processes and methods, because the problem is not solved solely by substituting materials. There are a large number of choices in the
2.3 Principles of Design 23implementation of the idea of light construction, especially in the area of design.The aim of a light-construction design is to increase the stiffness as far as possible,without any additional material. As regards stiffening, a distinction is made between: • beads • bottom boom members made of sections • shell-type design • forming of ribs • integration of beams • design of marginal reinforcements • bonding of metal foams. The most frequent application, in addition to beads, is the use of hollow sectionsversus solid sections. Apart from their lower weight per meter, they have higherbending and torsional stiffness, a good functional adjustment due to shaping, anda high capacity of integration. However, the forming operation is critical, withreference to the cross section and the longitudinal section, the distortion after theheat transfer during welding, the corrosion, and the compliance with the toleranceranges. Furthermore, a number of elastomechanic problems are to be taken intoconsideration, such as the application of forces, the ﬂow of forces in the shearcenter, and local or entire instability by buckling, tipping, and bulging. In the case of shell-type forming, the aim is to manufacture parts or sectionswith curved surfaces. Recently, sandwich designs have gained more and more importance. In themeantime, the ﬁrst serial applications have also taken place.2.3.3BionicsThe term bionics was ﬁrst used in 1960 by Major Jack E. Steele of the US Air Forceat a conference held in Dayton, Ohio. It is a combination of the words ‘biology’and ‘technics’, which means the use of biological principles for engineeringpurposes. The general idea of bionics is to decipher ‘inventions of the animatenature’, and their innovative application to engineering. Therefore, bionics is aninterdisciplinary subject where biologists, engineers and designers work together.Biological structures and organization are used either directly as a sample referredto as analogy bionics, or in an abstract way, detached from the biological archetype,referred to as abstraction bionics, and as an idea or an inspiration for solvingengineering problems. Although, there are some examples of the use of bionics inhistory, for example, the analysis and attempted transmission of the ﬂight of birdsonto ﬂying machines was performed by Leonardo da Vinci, nevertheless, bionicshas established itself as science only in the recent decades, primarily due to newand improved methods such as computer capacity and manufacturing processes. While developing functional elements from an engineering point of view, weshould be aware of the fact that parallel phenomena in nature have not always been